- Email: [email protected]

International Journal of Solids and Structures 44 (2007) 8119–8142 www.elsevier.com/locate/ijsolstr

Interlaminar hygrothermal stresses in laminated plates Arash Bahrami, Asghar Nosier

*

Department of Mechanical Engineering, Sharif University of Technology, P.O. Box 11365-9567, Azadi Avenue, Tehran, Iran Received 17 March 2007; received in revised form 31 May 2007 Available online 10 June 2007

Abstract Within the elasticity formulation the most general displacement ﬁeld for hygrothermal problems of long laminated composite plates is presented. The equivalent single-layer theories are then employed to determine the global deformation parameters appearing in the displacement ﬁelds of general cross-ply, symmetric, and antisymmetric angle-ply laminates under thermal and hygroscopic loadings. Reddy’s layerwise theory is subsequently used to determine the local deformation parameters of various displacement ﬁelds. An elasticity solution is also developed in order to validate the eﬃciency and accuracy of the layerwise theory in predicting the interlaminar normal and shear stress distributions. Finally, various numerical results are presented for edge-eﬀect problems of several cross-ply, symmetric, and antisymmetric angle-ply laminates subjected to uniform hygrothermal loads. All results indicate high stress gradients of interlaminar normal and shear stresses near the edges of laminates. 2007 Elsevier Ltd. All rights reserved. Keywords: Laminated plates; Interlaminar stresses; Elasticity formulation; Equivalent single-layer theories; Layerwise theory; Hygrothermal loading

1. Introduction With the ever-increasing applications of laminated composites in severe environmental conditions hygrothermal behavior of such laminates has attracted considerable attention. The interlaminar normal and shear stresses, on the other hand, are believed to play a signiﬁcant role in prediction of dominant cause of failure in composite laminates. These stresses that exhibit highly localized concentration near the edges of the laminate are the basis for damage in the form of free-edge delamination and the subsequent delamination growth in the interior region of laminates, leading to failure at loads below those corresponding to in plane failure. Therefore among the extensive research areas in the analysis of ﬁber-reinforced composites, the issue of interlaminar-edge stresses has been subject of tremendous investigations and various theoretical and experimental methods are employed to study the edge-eﬀect problem of composite laminates. Since, the present study is devoted to thermal and hygroscopic problems, in the proceeding only the pertinent works will be referred. A relatively comprehensive review of the various techniques of evaluation of interlaminar stresses that have *

Corresponding author. Tel.: +98 21 6616 5543; fax: +98 21 6600 0021. E-mail address: [email protected] (A. Nosier).

0020-7683/$ - see front matter 2007 Elsevier Ltd. All rights reserved. doi:10.1016/j.ijsolstr.2007.06.004

8120

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

appeared in the literature is available in the survey paper by Kant and Swaminathan (2000). Examination of the literature survey reveals that the ﬁrst paper considering the thermal loading in the edge-eﬀect problem of composite laminates is developed by Pagano (1974). He utilized a higher-order shear deformation theory (HSDT) to formulate the edge-eﬀect problem of symmetric balanced laminates subjected to a constant axial strain and a constant temperature change. Based on the formulation presented by Pipes and Pagano (1970), Wang and Crossman (1977a,b) studied the free-edge stresses in symmetric balanced laminates under a uniform thermal load using a ﬁnite element procedure. An approximate elasticity solution was presented by Wang and Choi (1982) to determine the boundary-layer stresses due to hygroscopic eﬀects. Wang and Chou (1989) obtained the transient interlaminar thermal stresses in symmetric balanced laminate by means of a zerothorder perturbation analysis of the equilibrium equations. Webber and Morton (1993) and Morton and Webber (1993) by following a similar approach to that used by Kassapoglou and Lagace (1986, 1987), attempted to calculate the interlaminar free-edge stress distribution in symmetric laminates subjected to thermal loads. By employing the complementary energy approach together with polynomial expansion of stress functions, Yin (1997) proposed a variational method to evaluate the thermal interlaminar stresses. Also Kim and Atlury (1995) developed an stress-based variational method to obtain interlaminar stresses under combined thermo-mechanical loading. In an eﬀort to determine the interlaminar stresses, an iterative technique in conjunction with the extended Kantorovich method is presented by Cho and Kim (2000) for thermal and mechanical loads. Rohwer et al. (2001) investigated the transverse shear and normal stresses in composite laminates subjected to thermal loading by using the extended two-dimensional method and the ﬁrst-order shear deformation plate theory (FSDT). A two-dimensional global higher-order deformation theory was proposed by Matsunaga (2004) for the calculation of out-of-plane stresses in cross-ply laminates subjected to thermal loading. Recently, a comprehensive examination of interlaminar stresses in general cross-ply laminates has been presented by Tahani and Nosier (2003, 2004). They used a layerwise theory to predict free-edge stresses in ﬁnite general cross-ply laminates under various mechanical, thermal, and hygroscopic loadings. Despite the intensive investigations on the analysis of interlaminar stresses in composite laminates, documented in the literature during the past three decades, few publications focused on the study of such stresses under hygrothermal loading conditions. In addition, for the case of hygrothermal loading, reliable numerical results are limited to cross-ply and symmetric balanced laminates. The purpose of the present work, however, is to analyze the interlaminar stresses in symmetric and unsymmetric cross-ply laminates, symmetric laminates, and antisymmetric angle-ply laminates subjected to uniform thermal and/or hygroscopic loadings. Towards this goal, both equivalent single-layer (ESL) and layerwise theories (LWT) are utilized. Each of the ESL and layerwise models has its advantages and disadvantages in terms of solution accuracy, solution economy, and simplicity. The ESL models which follow from an assumed global displacement ﬁeld lead to the deﬁnition of eﬀective overall rigidities and are incapable of providing precise calculation of local 3-D stress ﬁeld. On the other hand, the layerwise models which possess the ability of accurately describing the threedimensional eﬀects, such as free-edge stresses, are computationally expensive. Thus, it is attempted here to introduce a solution scheme which achieves maximum solution accuracy with minimal solution cost by employing an eﬃcient analytical procedure. This, on the other hand, is done by utilizing an appropriate ESL theory to determine the unknown constant parameters appearing in various laminates displacement ﬁelds. Interlaminar stresses are then determined by using an analysis based on the layerwise theory of Reddy. Lastly, an analytical elasticity solution is presented for a speciﬁc set of boundary and loading conditions in order to assess the eﬀectiveness and validity of the present developments. 2. Theoretical formulation The laminate considered in the present investigation is of thickness h, width 2b, and assumed to be long in the x-direction so that the strain components are functions of y and z only (Fig. 1). It is further assumed that the mechanical loads (if present) are applied at x = a and x = a only. Also the thermal and hygrothermal loadings are considered to be uniform everywhere in the laminate. Under these conditions the most general form of the displacement ﬁeld within the kth layer of the laminate has been shown to be as follows (Nosier and Bahrami, 2007; Lekhnitskii, 1981):

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8121

Fig. 1. Laminate geometry and coordinate system. ðkÞ

u1 ðx; y; zÞ ¼ B4 xy þ B6 xz þ B2 x þ uðkÞ ðy; zÞ 1 ðkÞ u2 ðx; y; zÞ ¼ B1 xz þ B3 x B4 x2 þ vðkÞ ðy; zÞ 2 1 ðkÞ u3 ðx; y; zÞ ¼ B1 xy þ B5 x B6 x2 þ wðkÞ ðy; zÞ 2 ðkÞ

ðkÞ

ð1Þ

ðkÞ

where, u1 ðx; y; zÞ, u2 ðx; y; zÞ, and u3 ðx; y; zÞ represent the displacement components in the x-, y-, and z-directions, respectively, of a material point initially located at (x, y, z) in the kth lamina of the laminate. It is next noted that as long as the loading conditions at x = a and x = a are similar (so that the laminate in Fig. 1 is globally in equilibrium), the following conditions will hold: ðkÞ

ðkÞ

ðkÞ

ðkÞ

u1 ðx; y; zÞ ¼ u1 ðx; y; zÞ u2 ðx; y; zÞ ¼ u2 ðx; y; zÞ ðkÞ u3 ðx; y; zÞ

¼

ð2Þ

ðkÞ u3 ðx; y; zÞ:

Upon imposing these restrictions on (1) it is readily seen that the constants B4 and B5 must vanish and the displacement ﬁeld in (1) is, therefore, reduced to what follows: ðkÞ

ð3aÞ

ðkÞ

ð3bÞ

ðkÞ

ð3cÞ

u1 ðx; y; zÞ ¼ B2 x þ B6 xz þ uðkÞ ðy; zÞ u2 ðx; y; zÞ ¼ B1 xz þ B3 x þ vðkÞ ðy; zÞ u3 ðx; y; zÞ ¼ B1 xy 12B6 x2 þ wðkÞ ðy; zÞ:

Furthermore, by replacing u(k)(y, z) appearing in (3a) by B3 y + u(k)(y, z), it becomes apparent that the terms involving B3 in (3) will generate no strains and, therefore, can be omitted (these terms, in fact, will correspond to an inﬁnitesimal rotation of the laminate about the z-axis in Fig. 1). Thus, the most general form of an arbitrary laminated composite laminate is given as follows: ðkÞ

ð4aÞ

ðkÞ

ð4bÞ

ðkÞ

ð4cÞ

u1 ðx; y; zÞ ¼ B2 x þ B6 xz þ uðkÞ ðy; zÞ u2 ðx; y; zÞ ¼ B1 xz þ vðkÞ ðy; zÞ u3 ðx; y; zÞ ¼ B1 xy 12B6 x2 þ wðkÞ ðy; zÞ:

The displacement ﬁeld in (4) may be used, in principle, for calculating the stress ﬁeld in any composite laminate subjected to arbitrary combinations of self-equilibrating mechanical and uniform hygrothermal loads. In the present study, however, our attention is focused on symmetric and unsymmetric cross-ply laminates, symmetric laminates, and antisymmetric angle-ply laminates subjected to uniform hygroscopic and thermal

8122

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

loadings. Since the solutions developed here in the present study signiﬁcantly depend on the lamination scheme, each of the aforementioned laminates is examined separately. 2.1. Cross-ply laminates For symmetric and unsymmetric cross-ply laminates (e.g., see Jones, 1998) subjected to uniform hygrothermal loadings, based on physical grounds, the following restrictions will, furthermore, hold (see Fig. 1): ðkÞ

ðkÞ

u1 ðx; y; zÞ ¼ u1 ðx; y; zÞ

ð5aÞ

ðkÞ u2 ðx; y; zÞ

ð5bÞ

¼

ðkÞ u2 ðx; y; zÞ:

Upon imposing (5a) on (4a) it is concluded that u(k)(y, z) = 0. Also from (5b) and (4b) it is concluded that B1 = 0. Thus, for cross-ply laminates the most general form of the displacement ﬁeld is given as follows: ðkÞ

u1 ðx; y; zÞ ¼ B2 x þ B6 xz ðkÞ

u2 ðx; y; zÞ ¼ vðkÞ ðy; zÞ 1 ðkÞ u3 ðx; y; zÞ ¼ B6 x2 þ wðkÞ ðy; zÞ: 2

ð6Þ

It is to be noted that for symmetric cross-ply laminates it can readily be shown that (see Eqs. (8) below) B6 = 0. 2.2. Symmetric laminates For symmetrically laminated composite plates (e.g., see Jones, 1998) under uniform hygrothermal loadings the deformational behavior of the material points within the laminates remains the same with respect to the middle surface. Thus, the following restrictions must hold with respect to the middle surface of any symmetric laminate with N layers: ðkÞ

ðNkþ1Þ

ðx; y; zÞ

ð7aÞ

ðkÞ

ðNkþ1Þ

ðx; y; zÞ:

ð7bÞ

u1 ðx; y; zÞ ¼ u1 u2 ðx; y; zÞ ¼ u2

From (7a) and (4a), it is concluded that B6 = 0. Also from (7b) and (4b) it is concluded that B1 = 0. Therefore, for symmetric laminates the most general form of the displacement ﬁeld is given as: ðkÞ

u1 ðx; y; zÞ ¼ B2 x þ uðkÞ ðy; zÞ ðkÞ

u2 ðx; y; zÞ ¼ vðkÞ ðy; zÞ ðkÞ u3 ðx; y; zÞ

ð8Þ

¼ wðkÞ ðy; zÞ:

2.3. Antisymmetric angle-ply laminates For antisymmetric angle-ply laminates with N layers (e.g., see Jones, 1998) subjected to uniform hygrothermal loadings the following condition must hold (see also Nosier and Bahrami, 2007): ðkÞ

ðNkþ1Þ

u1 ðx; y; zÞ ¼ u1

ðx; y; zÞ:

ð9Þ

From (9) and (4a) it is concluded that B6 = 0 and, therefore, the most general displacement ﬁeld for such laminates is given as follows: ðkÞ

u1 ðx; y; zÞ ¼ B2 x þ uðkÞ ðy; zÞ ðkÞ

u2 ðx; y; zÞ ¼ B1 xz þ vðkÞ ðy; zÞ ðkÞ

u3 ðx; y; zÞ ¼ B1 xy þ wðkÞ ðy; zÞ: The displacement ﬁelds in (6), (8), and (10) can be represented in one place as:

ð10Þ

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8123

ðkÞ

u1 ðx; y; zÞ ¼ B2 x þ dC B6 xz þ dAS uðkÞ ðy; zÞ ðkÞ

u2 ðx; y; zÞ ¼ dA B1 xz þ vðkÞ ðy; zÞ 1 ðkÞ u3 ðx; y; zÞ ¼ dA B1 xy dC B6 x2 þ wðkÞ ðy; zÞ 2

ð11Þ

where dA = dAS = 0 and dC = 1 for unsymmetric cross-ply laminates, dA = dC = 0 and dAS = 1 for symmetric laminates, and dA = dAS = 1 and dC = 0 for antisymmetric angle-ply laminates. It is to be noted that the terms involving the constant parameters B1, B2, and B6 describe the global deformations within the laminates whereas the functions u(k)(y, z), v(k)(y, z), and w(k)(y, z) correspond to the local deformations of kth layer within the laminate. 2.4. Equivalent single-layer theories It is well known by now that ESL theories are adequate in predicting the global responses of the composite laminates. On the other hand, these theories are simpler and computationally less time consuming than the layerwise theories. The objective of the present section is to present the simplest ESL theory which, on the other hand, will provide suﬃciently accurate results for the unknown constant parameters B1, B2, and B6 appearing in (11). For unsymmetric cross-ply and antisymmetric angle-ply laminates numerical studies conducted by the authors indicate the ﬁrst-order shear deformation theory of plates (FSDT), also known as Mindlin–Reissner plate theory, is fairly accurate in predicting these parameters. For symmetric laminates, however, an improved ﬁrst-order theory must be developed and used for determining the appropriate constant parameter (i.e., B2) appearing in the displacement ﬁeld (11). In FSDT the components of the displacement vector at a material point in the laminate are expressed in the following form (Reddy, 2003): u1 ðx; y; zÞ ¼ uðx; yÞ þ zwx ðx; yÞ u2 ðx; y; zÞ ¼ vðx; yÞ þ zwy ðx; yÞ

ð12Þ

u3 ðx; y; zÞ ¼ wðx; yÞ where u, v, and w denote the displacements of a point located on the middle plane of the laminate. Also wx and wy are the rotations of transverse normals about the y- and x-axes, respectively. The displacement ﬁeld in (6) indicates that for hygrothermal problems of cross-ply laminates the displacement ﬁeld within FSDT (i.e., Eq. (12)) must take the following simpler form: u1 ðx; y; zÞ ¼ B2 x þ B6 xz u2 ðx; y; zÞ ¼ V ðyÞ þ zWy ðyÞ

ð13Þ

u3 ðx; y; zÞ ¼ 12B6 x2 þ W ðyÞ with B6 being equal to zero when the cross-ply laminate is symmetric. Similarly, based on the displacement ﬁeld in (10), it is concluded that for hygrothermal problems of antisymmetric angle-ply laminates the displacement ﬁeld within FSDT must take the following simpler form: u1 ðx; y; zÞ ¼ B2 x þ U ðyÞ þ zWx ðyÞ u2 ðx; y; zÞ ¼ B1 xz þ V ðyÞ þ zWy ðyÞ

ð14Þ

u3 ðx; y; zÞ ¼ B1 xy þ W ðyÞ: As it is pointed out earlier, for symmetric laminates FSDT is incapable of accurately determining the unknown parameter B2 appearing in (8). This is attributed to the fact that, when such laminates are subjected to uniform hygrothermal loads, the unknown functions wx, wy, and w vanish and the remaining terms in (12) will not be adequate for accurate determination of B2. On the other hand, in symmetric laminates under hygrothermal loadings the displacement components u1, u2 must be even functions of thickness coordinate z whereas u3 must be an odd function of z. For such laminates it is found that a more accurate result for B2 may be found by introducing the following displacement ﬁeld:

8124

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

~ x ðx; yÞ u1 ðx; y; zÞ ¼ uðx; yÞ þ jzjw ~ y ðx; yÞ u2 ðx; y; zÞ ¼ vðx; yÞ þ jzjw

ð15Þ

u3 ðx; y; zÞ ¼ zwz ðx; yÞ: Numerical studies reveal, furthermore, that the thickness stretching term (i.e., zwz) introduced in (15) has a negligible eﬀect on the accuracy of B2 and, therefore, can be omitted when symmetric laminates are subjected to uniform hygrothermal loadings. Based on the displacement ﬁeld in (8), it is, thus, concluded that the simplest appropriate displacement ﬁeld for symmetric laminates is given as follows: ~ x ðyÞ u1 ðx; y; zÞ ¼ B2 x þ U ðyÞ þ jzjW ~ y ðyÞ u2 ðx; y; zÞ ¼ V ðyÞ þ jzjW

ð16Þ

u3 ðx; y; zÞ ¼ 0: The theory that will be developed here using (16) will be referred to as the improved ﬁrst-order shear deformation plate theory (IFSDT). It remains to ﬁnd and, thereafter, solve the equilibrium equations corresponding to the displacement ﬁelds in Eqs. (13), (14), and (16) in order to determine the constant parameters existing in these displacement ﬁelds. For brevity, however, here the detail of the procedure is demonstrated for the displacement ﬁeld in (16) only and the results corresponding to the displacement ﬁelds in (13) and (14) are summarized. By using the displacement ﬁeld (16) in the principle of minimum total potential energy (Fung and Tong, 2001) and treating the constant B2 as an unknown parameter ﬁve equilibrium equations are obtained which may be presented as follows: dU : N 0xy ¼ 0

ð17aÞ

dV : N 0y ¼ 0

ð17bÞ

~ 0 xy ¼ 0 ~x M ~x : Q dW

ð17cÞ

~ 0y ¼ 0 ~y M ~y : Q dW

ð17dÞ

Z

b

dB2 :

N x dy ¼ 0

ð18Þ

b

where a prime indicates an ordinary diﬀerentiation with respect to variable y and the stress and moment resultants appearing in (17) and (18) are deﬁned as follows: Z h=2 Z h=2 ~ x; Q ~yÞ ¼ ðN x ; N y ; N xy Þ ¼ ðrx ; ry ; rxy Þ dz; ðQ sgnðzÞðrxz ; ryz Þ dz ~ y; M ~ xy Þ ¼ ðM

Z

h=2

h=2

h=2

jzjðry ; rxy Þ dz

ð19aÞ

h=2

with sgnðzÞ ¼

1 for z < 0 1 for z > 0:

ð19bÞ

Upon substitution of the displacement ﬁeld (16) into Eq. (19a), through the linear strain-displacement relations of elasticity and the plane-stress constitutive law (Herakovich, 1998) of a lamina, the stress and moment resultants may be expressed as:

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8 Nx > > > > > > < Ny

9 > > > > > > =

2

A16

A12

6 6 A26 6 N xy ¼6 A66 > 6 > > 6~ > > ~y > M > > 4 B26 > > > ; :~ > ~ 66 M xy B and

(

~y Q ~ Qx

) ¼k

2

~ 16 B ~ 26 B

~ 12 B ~ 22 B

A22 A26 ~ 22 B

~ 66 B

~ 26 B

D26

D22

~ 26 B

D66

D26

8 H 9 Nx > > > > > > > NH > > > > > > = < y > H N xy > > > > > > > > ~H> > > > M > > > y > > > > > ; : ~H> ; M xy xy

38 0 9 8 N T > x A11 > > > > >U > > > T > > > 7> 0 > N > > >V > A12 7< = > < y 7 ~0 NT A16 7 7> Wx > > xy > > ~0 > > ~T ~ 12 7 Wy > > > > 5> M B > > > y > > > ; > : : ~T ~ 16 B2 B M

9 > > > > > > > =

( ~ ) Wy ~x A55 W

A44

A45

A45

8125

ð20aÞ

ð20bÞ

~ ij , and Dij are deﬁned as: where the laminate rigidities Aij, B Z h=2 ij ð1; jzj; z2 Þ dz ~ ij ; Dij Þ ¼ ðAij ; B Q

ð21Þ

h=2

ij being the transformed reduced stiﬀness (Herakovich, 1998) of an orthotropic lamina. Also NT, M ~ T are with Q referred to as the thermal resultants and deﬁned as: Z h=2 h i T T T 12 ; Q 16 Þax þ ðQ 12 ; Q 22 ; Q 26 Þay þ ðQ 16 ; Q 26 ; Q 66 Þaxy DT dz 11 ; Q ðN x ; N y ; N xy Þ ¼ ðQ ð22aÞ h=2

~TÞ ¼ ~ T; M ðM y xy

Z

h=2

h

i 16 Þax þ ðQ 22 ; Q 26 Þay þ ðQ 26 ; Q 66 Þaxy DT jzj dz 12 ; Q ðQ

ð22bÞ

h=2

where DT denotes the temperature change and ax, ay, and axy denote the transformed coeﬃcients of thermal expansions (Herakovich, 1998). The hygroscopic resultants are, similarly, deﬁned as: Z h=2 h i H H 12 ; Q 16 Þbx þ ðQ 12 ; Q 22 ; Q 26 Þby þ ðQ 16 ; Q 26 ; Q 66 Þbxy DM dz 11 ; Q ðN H ; N ; N Þ ¼ ðQ ð23aÞ x y xy h=2

~ HÞ ¼ ~ H; M ðM y xy

Z

h=2

h

i 16 Þbx þ ðQ 22 ; Q 26 Þby þ ðQ 26 ; Q 66 Þbxy DMjzj dz: 12 ; Q ðQ

ð23bÞ

h=2

In Eqs. (23), DM is the percent moisture (by weight) absorbed by each layer in the laminate and bx, by, and bxy indicate the transformed coeﬃcients of hygroscopic expansions (Herakovich, 1998). Also in (20b) the constant k2 is called the shear correction factor which is often introduced for in a ﬁrst-order theory to modify the laminate transverse shear rigidities. For free edges of the laminate at y = ±b according to the principle of minimum total potential energy the following traction-free boundary conditions must be imposed: N y ¼ N xy ¼ 0

at y ¼ b

ð24aÞ

and ~ xy ¼ M ~y ¼ 0 M

at y ¼ b:

ð24bÞ

Integrating the equilibrium equations in (17a) and (17b) and imposing the boundary conditions in (24a) yield: N y ðyÞ ¼ N xy ðyÞ ¼ 0:

ð25Þ

~ x and W ~ y , and B2. This way the These conditions are used to express U and V appearing in (20a) in terms of W ~ x and W ~ y , and B2. Finally, upon substitution of M ~ y , and M ~ xy are all expressed in terms of W ~ xy resultants Nx, M ~ y , and (20b) into the equilibrium equations (17c) and (17d), the following results are obtained: and M 0

0

~ 00 k 2 A55 W ~x þ D ~ 00 k 2 A45 W ~y ¼ 0 ~x : D 66 W 26 W dW x y ~y : dW

~ 00 26 W D x

~x þ k A45 W 2

~ 00 22 W D y

~y ¼ 0 k A44 W 2

ð26aÞ ð26bÞ

8126

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

22 , D 26 , and D 66 being displayed in Appendix A. Upon imposing the boundary conditions with the coeﬃcients D ~ x and W ~ y are obtained in in (24b) on the general solution of (26), the generalized displacement functions W terms of the unknown constant B2 which, on the other hand, may be presented as follows: ~ x ðyÞ ¼ W

2 X

Aj sinhðkj yÞ;

~ y ðyÞ ¼ W

j¼1

2 X

j Aj sinhðkj yÞ D

ð27Þ

j¼1

j ðj ¼ 1; 2Þ are given as: where the coeﬃcients Aj and D A1 ¼ d 1 B2 þ mTy þ mH y

ð28aÞ

A2 ¼ d 2 B2 þ mTxy þ mH xy

ð28bÞ

j ¼ D

66 k2 k 2 A55 D j ðj ¼ 1; 2Þ: 26 k2 k 2 A45 D

ð28cÞ

j

The constant parameters appearing in (28a) and (28b) are presented in Appendix A. In addition, k2j (j = 1, 2) appearing in (28c) are the roots of the following characteristic equation (associated with Eqs. (26)): 2

66 k 2 A55 Þðk2 D 22 k 2 A44 Þ ðk2 D 26 k 2 A45 Þ ¼ 0: ðk2 D

ð29Þ

Finally, upon substituting (27) into the stress resultant Nx and the subsequent result into the global equilibrium equation (18), the constant parameter B2 is determined which, on the other hand, may be presented as follows: 1 B2 ¼ ðnTx þ nH x Þ ^ h

ð30Þ

where the expressions for ^ h, nTx , and nH x are also listed in Appendix A. It is remarked earlier that a procedure similar to that outlined here for symmetric laminates may be employed to determine the unknown parameters appearing in the displacement ﬁelds of unsymmetric crossply and antisymmetric angle-ply laminates. For brevity, however, only the appropriate results are presented here. For cross-ply laminates the constants B2 and B6 appearing in (13) are found to be as follows: T T 1 H h4 nx þ nH B2 ¼ ð31aÞ x h2 m x þ m x h1 h4 h2 h3 T T 1 H : ð31bÞ B6 ¼ h1 mx þ mH x h3 nx þ nx h1 h4 h2 h3 The expressions for the constant parameters appearing in (31) are for clarity displayed in Appendix B. For antisymmetric angle-ply laminates the constants parameters B1 and B2 appearing in the displacement ﬁeld (14) are found to be as follows: h

i 1 T H h4 nTx þ nH m þ m B1 ¼ ð32aÞ h 2 x xy xy h1 h4 h2 h3

h T i 1 H h1 mTxy þ mH B2 ¼ : ð32bÞ xy h3 nx þ nx h1 h4 h2 h3 The constant parameters in (32) are listed in Appendix C. 2.5. Layerwise laminated plate theory of Reddy Due to existence of local high stress gradient and the three-dimensional nature of the boundary-layer phenomenon, the interlaminar stresses in the boundary-layer regions can not be computed accurately by the ESL theories. Thus, Reddy’s layerwise theory that is capable of modeling localized three-dimensional eﬀects is utilized here to carry out the hygrothermal interlaminar stress analysis in laminates with free edges. The theory assumes that the displacement components of a generic point in the laminate are given by (Nosier et al., 1993):

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

u1 ðx; y; zÞ ¼ uk ðx; yÞUk ðzÞ u2 ðx; y; zÞ ¼ vk ðx; yÞUk ðzÞ k ¼ 1; 2; . . . ; N þ 1

8127

ð33Þ

u3 ðx; y; zÞ ¼ wk ðx; yÞUk ðzÞ with k being a dummy index indicating summation from 1 to N + 1. In (33) u1, u2, and u3 denote the displacement components in the x-, y-, and z-directions, respectively, of a material point located at (x, y, z) in the undeformed state. Also, uk(x, y), vk(x, y), and wk(x, y) indicate the displacements of all points located, initially, on the kth plane in the x-, y-, and z-directions, respectively. In addition, N corresponds to the total number of numerical layers considered in a laminate. Furthermore, Uk(z) are the global Lagrangian interpolation polynomials associated with the kth surface (see Tahani and Nosier, 2004; Reddy, 2003; Nosier et al., 1993). It is to be noted that the layerwise concept introduced here is very general in a sense that the accuracy of the solution can be improved as close as desired by increasing the number of the subdivisions through the thickness or increasing the order of interpolation polynomials through the thickness. However, in the present study, the interpolation functions Uk(z) are assumed to have linear variation through the thickness of each numerical layer. The elasticity-based displacement ﬁeld in (11) indicates that the displacement ﬁeld of LWT appearing in (33) must be rewritten in a simpler form as follows: u1 ðx; y; zÞ ¼ B2 x þ dC B6 xz þ dAS U k ðyÞUk ðzÞ u2 ðx; y; zÞ ¼ dA B1 xz þ V k ðyÞUk ðzÞ u3 ðx; y; zÞ ¼ dA B1 xy

1 d B x2 2 C 6

k ¼ 1; 2; . . . ; N þ 1

ð34Þ

þ W k ðyÞUk ðzÞ:

Substitution of (34) into the linear strain–displacement relations of elasticity (e.g., see Fung and Tong, 2001) yields the following results: ey ¼ V 0k Uk ;

ex ¼ B2 þ dC B6 z;

cxz ¼ dAS U k U0k þ dA B1 y;

ez ¼ W k U0k ;

cyz ¼ W 0k Uk þ V k U0k

cxy ¼ dAS U 0k Uk dA B1 z:

ð35Þ

The equilibrium equations of a laminate within LWT are obtained employing (35) in the principle of minimum potential energy (e.g., see Fung and Tong, 2001). The results are, in general, 3(N + 1) local equilibrium equations corresponding to 3(N + 1) unknown functions Uk, Vk, and Wk, and three global equations corresponding to the three unknown constants B1, B2, and B6 as follows: ! dM kxy k dU k : dAS Qx ¼0 ð36aÞ dy dV k : Qky

dM ky ¼0 dy

dRky ¼0 dy Z h=2 Z b dB1 : dA ðrxz y rxy zÞ dy dz ¼ 0 dW k : N kz

h=2

Z

h=2

Z

Z

ð36cÞ ð37aÞ

b b

rx dy dz ¼ 0

dB2 : h=2

ð36bÞ

ð37bÞ

b h=2

Z

b

dB6 : dC h=2

rx z dy dz ¼ 0:

b

Here, the generalized stress resultants, appearing in Eqs. (36a) through (36c), are deﬁned as:

ð37cÞ

8128

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

ðM ky ; M kxy ; N kz Þ ¼ ðQkx ; Qky ; Rky Þ

¼

Z

Z

h=2

h=2

ðry Uk ; rxy Uk ; rz U0k Þ dz ð38Þ

h=2

h=2

ðrxz U0k ; ryz U0k ; ryz Uk Þ dz:

It is next noted that the three-dimensional stress–strain relations within the kth layer of composite laminate are given as (e.g., see Herakovich, 1998): ðkÞ ðkÞ feg feT g feH g ðkÞ ð39Þ frg ¼ ½C being the transformed stiﬀness matrix and {eT} and {eH} being the thermal and hygroscopic strains, with ½C respectively. By merely substituting relations (35) into (39) and the subsequent results into (38), the generalized stress resultants are expressed in terms of the displacement functions: kj jk kj kj jk kj kj kj 0 0 ðM ky ; M kxy ; N kz Þ ¼ dAS ðDkj 26 ; D66 ; B36 ÞU j þ ðD22 ; D26 ; B23 ÞV j þ ðB23 ; B36 ; A33 ÞW j k ÞB1 þ dC ðDk ; Dk ; B k ÞB6 þ ðBk ; Bk ; Ak ÞB2 dA ðDk ; Dk ; B 12

16

13

26

66

36

12

16

13

kðTÞ kðHÞ ðM kðTÞ ; M kðTÞ Þ ðM kðHÞ ; M kðHÞ Þ y xy ; N z y xy ; N z

ð40Þ

kj kj kj kj kj jk jk kj 0 ðQkx ; Qky ; Rky Þ ¼ dAS ðAkj 55 ; A45 ; B45 ÞU j þ ðA45 ; A44 ; B44 ÞV j þ ðB45 ; B44 ; D44 ÞW j

þ dA ðAk55 ; Ak45 ; Bk45 ÞB1 y where the expressions for laminate rigidities and the thermal and hygroscopic resultants are listed in Appendix D. Lastly, upon substitution of Eqs. (40) into (36) and (37), the governing equations of equilibrium are obtained in the following form: h i kj kj 00 kj kj jk k 00 0 dU k : dAS Dkj ð41aÞ 66 U j A55 U j þ D26 V j A45 V j þ ðB36 B45 ÞW j ¼ dA B1 A55 y kj kj 00 kj kj jk k 00 0 dV k : dAS Dkj 26 U j dAS A45 U j þ D22 V j A44 V j þ ðB23 B44 ÞW j ¼ dA B1 A45 y jk kj jk kj kj 0 0 00 dW k : dAS ðBkj 45 B36 ÞU j þ ðB44 B23 ÞV j þ D44 W j A33 W j k B6 N kðTÞ N kðHÞ k Þ þ dC B ¼ B2 Ak13 dA B1 ðBk45 þ B 36 13 z z Z bh j36 W j Þ dB1 : dA ðdAS Aj55 U j þ Aj45 V j þ Bj45 W 0j Þy ðdAS Dj66 U 0j þ Dj26 V 0j þ B b i þ dA B1 ðA55 y 2 þ D66 Þ B2 B16 dC B6 D16 þ M Txy þ M Hxy dy ¼ 0 Z bh i dB2 : dAS Bj16 U 0j þ Bj12 V 0j þ Aj13 W j þ B2 A11 þ dC B6 B11 dA B1 B16 N Tx N Hx dy ¼ 0

ð41bÞ

ð41cÞ

ð42aÞ ð42bÞ

b

Z

b

dB6 : dC b

h i j13 W j þ B2 B11 þ dC B6 D11 dA B1 D16 M T M H dy ¼ 0: dAS Dj16 U 0j þ Dj12 V 0j þ B x x

ð42cÞ

To investigate the free-edge-eﬀect problem, Eqs. (41) and (42) must be solved subject to the following tractionfree boundary conditions at y = ±b: dAS M kxy ¼ M ky ¼ Rky ¼ 0

at y ¼ b:

ð43Þ

As it is seen from (41) the local displacement equations comprise of 3(N + 1) coupled second-order diﬀerential equations with constant coeﬃcients. It is clear that such a linear system may be solved analytically using, for example, the state space approach. This way, the displacement components will be found, in general, in terms of B1, B2, B6, and 6(N + 1) constants of integration. Three global displacement equations in (42) and 6(N + 1) boundary conditions in (43) are, then, employed to determine integration constants and unknown coeﬃcients B1, B2, and B6. A detailed description of the solution scheme has been presented in Nosier and Bahrami (2006, 2007) and, therefore, for brevity will not be repeated here. It is to be noted that the constant parameters B1, B2, and B6 appearing in (34) may be considered to be known from an analysis based on the ﬁrst-order theories

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8129

developed here (see Eqs. (30) through (32)) since they represent global response quantities of laminates. In fact the accuracy of the ﬁrst-order theories in predicting these parameters will be assessed within the present study when numerical results are discussed. 2.6. Theory of elasticity In order to verify the validity of the solutions obtained in the previous sections, an analytical elasticity solution is presented here for particular boundary and loading conditions. A generally stacked laminate subjected to a uniform hygrothermal loading is considered. It is, moreover, assumed that the ends of the laminate in Fig. 1 are gripped so that the line AB (EF) is not allowed to have rotations about the x-axis and the line cc (the x-axis and the line dd). Under such assumptions the constants B1 and B6 vanish and the displacement ﬁeld of elasticity in (4) is simpliﬁed to what follows: ðkÞ

u1 ðx; y; zÞ ¼ B2 x þ uðkÞ ðy; zÞ ðkÞ

u2 ðx; y; zÞ ¼ vðkÞ ðy; zÞ ðkÞ u3 ðx; y; zÞ

ð44Þ

ðkÞ

¼ w ðy; zÞ:

The constant B2 appearing in (44) represents the uniform axial strain in the x-direction due to a hygrothermal loading and will be determined here within the elasticity theory. By employing the displacement ﬁeld (44) in the principle of minimum total potential energy (e.g., see Fung and Tong, 2001) the local and global equilibrium equations are readily found to be: du :

orðkÞ orðkÞ xy þ xz ¼ 0 oy oz

ð45aÞ

dv :

orðkÞ orðkÞ y yz þ ¼0 oy oz

ð45bÞ

dw :

orðkÞ orðkÞ yz þ z ¼0 oy oz

ð45cÞ

and Z

b

Z

h=2

rx dz dy ¼ 0;

dB2 : b

ð46Þ

h=2

respectively. For traction-free boundary conditions at y = ±b, no analytical solution seems to exist for Eqs. (45a) through (45c). It is, however, noted that Eqs. (45) admit an analytical solution for the following boundary conditions at y = ±b: ðkÞ

ðkÞ rðkÞ y ¼ u3 ¼ rxy ¼ 0

at y ¼ b:

ð47Þ

Using the three-dimensional stress–strain relations in (39) together with strain-displacement relationships of elasticity (e.g., see Fung and Tong, 2001), the local equilibrium equations in (45) may be expressed in terms of the displacement components as follows: ðkÞ uðkÞ þ C ðkÞ uðkÞ þ C ðkÞ vðkÞ þ C ðkÞ vðkÞ þ ðC ðkÞ þ C ðkÞ ÞwðkÞ ¼ 0 C 55 ;zz 66 ;yy 26 ;yy 45 ;zz 45 36 ;yz ðkÞ uðkÞ þ C ðkÞ vðkÞ þ C ðkÞ vðkÞ þ ðC ðkÞ þ C ðkÞ ÞwðkÞ ¼ 0 ðkÞ uðkÞ þ C C 26 ;yy 45 ;zz 22 ;yy 44 ;zz 23 44 ;yz ðkÞ ðC 45

þ

ðkÞ ÞuðkÞ C 36 ;yz

þ

ðkÞ ðC 23

þ

ðkÞ ÞvðkÞ C 44 ;yz

þ

ðkÞ wðkÞ C 44 ;yy

þ

ðkÞ wðkÞ C 33 ;zz

ð48Þ

¼0

where a coma followed by a variable denotes partial diﬀerentiation with respect to that variable. Similarly, the boundary conditions in (47) are expressed in terms of the displacement components as follows:

8130

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

ðkÞ vðkÞ þ C ðkÞ wðkÞ ¼ C ðkÞ ðekðTÞ þ ekðHÞ B2 Þ ðkÞ uðkÞ þ C C 26 ;y 22 ;y 23 ;z 12 x x ðkÞ ðekðTÞ þ ekðHÞ Þ þ C ðkÞ ðckðTÞ þ ckðHÞ Þ ðkÞ ðekðTÞ þ ekðHÞ Þ þ C þC 22 23 26 y y z z xy xy ðkÞ uðkÞ þ C ðkÞ vðkÞ þ C ðkÞ wðkÞ ¼ C ðkÞ ðekðTÞ þ ekðHÞ B2 Þ at y ¼ b C 66 ;y 26 ;y 36 ;z 16 x x

ð49Þ

ðkÞ ðekðTÞ þ ekðHÞ Þ þ C ðkÞ ðckðTÞ þ ckðHÞ Þ ðkÞ ðekðTÞ þ ekðHÞ Þ þ C þC 26 36 66 y y z z xy xy wðkÞ ¼ 0: It remains next to obtain the solution of Eqs. (48) satisfying the boundary conditions in (49) and the following conditions: The traction-free conditions at the top surface of the ﬁrst layer: ð1Þ ð1Þ rð1Þ z ¼ ryz ¼ rxz ¼ 0 at the top surface of the 1st layer:

ð50aÞ

The traction-free conditions at the bottom surface of the Nth layer: Þ ðN Þ ðN Þ ¼ ryz ¼ rxz ¼ 0 at the bottom surface of the N th layer: rðN z

ð50bÞ

The displacement continuity conditions at every interface within the laminate: ðkÞ

ðkþ1Þ

u1 ¼ u1

ðkÞ

ðkþ1Þ

; u2 ¼ u 2

ðkÞ

ðkþ1Þ

; and u3 ¼ u3

ð50cÞ

at interfaces:

The stress equilibrium conditions at every interface within the laminate: ðkþ1Þ ðkþ1Þ ðkþ1Þ ; rðkÞ ; and rðkÞ at interfaces: rðkÞ z ¼ rz yz ¼ ryz xz ¼ rxz

ð50dÞ

Eqs. (48) with the boundary conditions in (49) may be solved by means of the Fourier series technique. A complete description of the solution procedure is discussed in Nosier and Bahrami (2007) and, for the sake of brevity, is not repeated here. The displacement components within the kth layer of the laminate are found to be: ðkÞ

u1 ðx; y; zÞ ¼ B2 x þ

1 X 6 X

Akmi ekkmi z sinðam yÞ þ

m¼0 i¼1 ðkÞ

u2 ðx; y; zÞ ¼

1 X 6 X

ðkÞ

Akm sinðam yÞ

m¼1

kmi Akmi ekkmi z sinðam yÞ þ B

m¼0 i¼1

u3 ðx; y; zÞ ¼

1 X

1 X

Bkm sinðam yÞ

ð51Þ

m¼1

1 X 6 X

kmi Akmi ekkmi z cosðam yÞ C

m¼0 i¼1

where am = (2m + 1)p/2b equation: ðkÞ a2 C ðkÞ k2 m 66 þ C 55 km ðkÞ ðkÞ 2 a2 C þ C m 26 45 kkm ðkÞ am kkm ðC þC ðkÞ Þ 45 36

and kkmi (i = 1, 2, . . . , 6) are the roots of the following sixth-order polynomial ðkÞ þ C ðkÞ Þ am kkm ðC 45 36 ðkÞ þ C ðkÞ Þ ¼ 0: am kkm ðC 44 23 m 22 km 44 2 ðkÞ ðkÞ þ C ðkÞ Þ a2 C ðkÞ am kkm ðC 44 23 m 44 þ kkm C 33

ðkÞ þ k2 C ðkÞ a2m C 26 km 45 ðkÞ þ k2 C ðkÞ a2 C

ð52Þ

Also the parameters Akm and Bkm appearing in (51) are given by: Akm ¼

ðkÞ C ðkÞ ðkÞ ðkÞ C 12 26 C 16 C 22 B2 a m 2 ðkÞ ðkÞ C ðkÞ C C 66

22

26

and

Bkm ¼

ðkÞ C ðkÞ ðkÞ ðkÞ C 16 26 C 12 C 66 B2 a m 2 ðkÞ ðkÞ C ðkÞ C C 66

22

ð53aÞ

26

with am ¼

8b ð1Þm : p2 ð2m þ 1Þ2

kmi appearing in (51) are determined from the following relations: kmi and C Moreover, the coeﬃcients B

ð53bÞ

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

" 2 ðkÞ ðkÞ am C 26 þ k2kmi C Bkmi 45 ¼ kmi ðkÞ þ k2 C ðkÞ C a2m C 22 kmi 44

ðkÞ þ C ðkÞ Þ am kkmi ðC 45 36 ðkÞ þ C ðkÞ Þ am kkmi ðC 44

#1 (

23

ðkÞ C ðkÞ k2 a2m C 55 kmi 66 ðkÞ C ðkÞ k2 a2 C m

26

45

8131

) ð54Þ

:

kmi

The next step of the analysis is to determine the 6N unknowns, namely, Akmi (k = 1, 2, . . . , N and i = 1, . . . , 6) for each Fourier integer m and the unknown parameter B2. These unknowns will be determined in a try and error process by imposing the conditions in (50a) through (50d) and Eq. (46). For this purpose, an initial value is assumed for B2. This value is then substituted into conditions (50a) through (50d) to obtain a system of 6N algebraic equations in terms of Akmi (for each m) which upon solving yields the unknown coeﬃcients Akmi (k = 1, 2, . . . , N and i = 1, . . . , 6). Next, upon carrying out the integration in (46) a new B2 is found which, on the other hand, may be presented as: 2 3 N P 1 P ðkÞ ðkÞ m T H hk ðC 12 Bkm þ C 16 Akm Þð1Þ 6 bðN x þ N x Þ 7 1 k¼1 m¼1 6 7 B2 ¼ PN ðkÞ 6 ð55Þ

7 N P 1 P 6 hk 4 5 ðkÞ þC kmi C ðkÞ ðkÞ P kmi C C B b k¼1 C m kkmi hk 12 16 13 11 2 þ am Akmi ð1Þ sinhð 2 Þ kkmi k¼1 m¼0 i¼1

where

N Tx

and

N Tx ¼

NH x

appearing in (55) are deﬁned as:

N X ðkÞ aðkÞ þ C ðkÞ aðkÞ þ C ðkÞ aðkÞ þ C ðkÞ aðkÞ Þhk DT ðC 11 x 12 y 13 z 16 xy k¼1

ð56Þ

N X ðkÞ bðkÞ þ C ðkÞ bðkÞ þ C ðkÞ bðkÞ þ C ðkÞ bðkÞ Þhk DM: NH ðC 11 x 12 y 13 z 16 xy x ¼ k¼1

It is reminded here that for convenience the z coordinate is located at the middle surface of each ply. The new value of B2 is then compared with that assumed initially. If the diﬀerence between two values is signiﬁcant, the new value of B2 in (55) is used as the initial value and the procedure is repeated until B2 is obtained with any desirable degree of accuracy. It is to be noted that by substituting B2 into (53a) and subsequent results into (51) the displacement components will be obtained. Upon substitution of the displacement ﬁeld into strain-displacement relations of linear elasticity (e.g., see Fung and Tong, 2001) and using the three-dimensional Hooke law (39) the stress components are ﬁnally determined. It is pointed out that the elasticity solution presented here is, although analytical, not an exact solution since the Gibbs phenomenon appears in the Fourier expansions introduced in the solution procedure (see Nosier and Bahrami, 2007). In fact, according to the solution obtained here, the interlaminar normal stress rz will vanish at points located on the edges of the laminate at y = ±b which is not a correct result. The exact value of rz on these edges may, however, be determined by considering the following three-dimensional strain–stress relations (e.g., see Herakovich, 1998): ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ eðkÞ x ¼ S 11 rx þ S 12 ry þ S 13 rz þ S 16 rxy þ ax DT þ bx DM ðkÞ

ðkÞ

ðkÞ

ð57Þ

ðkÞ

ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ eðkÞ z ¼ S 13 rx þ S 23 ry þ S 33 rz þ S 36 rxy þ az DT þ bz DM ðkÞ

ðkÞ

where Sij ’s are the oﬀ-axis compliances of the kth layer. At the edges of the laminate u3 is speciﬁed to vanish (see (47)). Therefore, at all points on these edges (except for points located at the intersections of these edges with interfaces, bottom surface, and top surface of the laminate) it can be concluded: ðkÞ

ez

ou3 ¼0 oz

at y ¼ b:

ð58Þ

Next, substitution of (47) and (58) (and eðkÞ x ¼ B2 ) into (57) results in: ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ B2 ¼ S11 rðkÞ x þ S 13 rz þ ax DT þ bx DM

0¼

ðkÞ S13 rðkÞ x

þ

ðkÞ S33 rðkÞ z

ð59aÞ

ðkÞ þ aðkÞ z DT þ bz DM:

Upon solving Eqs. (59) the exact value of

rðkÞ z

ð59bÞ is obtained to be as follows:

8132

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

rðkÞ z ¼

ðkÞ ðkÞ ðkÞ ðkÞ ðkÞ S11 ðaðkÞ z DT þ bz DMÞ þ S 13 ðB2 ax DT bx DMÞ : ðkÞ2 ðkÞ ðkÞ S S S 13

11

ð60Þ

33

Relation (60) indicates that the interlaminar normal stress rðkÞ z has a constant value at the edges of each lamina (at y = ±b) and, in addition, this constant value changes from one layer to another (adjacent) layer because of changes in ﬁber orientations. 3. Numerical results and discussions In this section the validity and accuracy of the theories and procedures introduced here in the present study are ﬁrst assessed trough several numerical examples by considering cross-ply laminates with special boundary conditions (47) at y = ±b. For this purpose numerical results of ESL and layerwise theories for a uniform temperature change are compared with those of elasticity theory. The interlaminar stresses within various crossply, symmetric, and antisymmetric angle-ply laminates with free edges at y = ±b are then closely examined. The material layers within any laminate are assumed to have identical thickness (hk), density, and on-axis properties. The mechanical and thermal properties of each lamina are, furthermore, assumed to be the same as those of graphite/epoxy T300/5208 (Herakovich, 1998): E1 ¼ 132 GPa; E2 ¼ E3 ¼ 10:8 GPa; m12 ¼ m13 ¼ 0:24;

m23 ¼ 0:59;

G12 ¼ G13 ¼ 5:65 GPa; G23 ¼ 3:38 GPa;

a1 ¼ 0:77 106 =C ;

ð61Þ

a2 ¼ a3 ¼ 0:25 106 =C :

Moreover, the thickness of each physical lamina is assumed to be 1 mm (i.e., hk = 1 mm). In addition, since the responses of various laminates due to thermal and hygroscopic loads are similar, only thermal results (due to a uniform temperature change DT = 1 C) are presented here. Furthermore, in the numerical examples the value 5/6 is used for the shear correction factor, k2, in the ﬁrst-order plate theories and the interlaminar stress components according to LWT are computed by integrating the local equilibrium equations of elasticity (see, e.g., Reddy, 2003). Numerical values of B2 according to FSDT, IFSDT, LWT, and elasticity theory are listed in Table 1 for cross-ply [90/0/0/90] and [0/90/0/90] laminates with boundary conditions in (47) under the uniform thermal load DT = 1 C. The ratio of the laminate width to its thickness is assumed to be 5 (i.e., 2b/h = 5) for the numerical results in Table 1. It is observed that the layerwise theory overestimates the numerical values of B2 and by, however, increasing the number of numerical layers (p) in each physical layer (see Tahani and Nosier, 2004; Nosier et al., 1993) the results of LWT approach those of the elasticity theory. It is to be noted that the numerical values of B2 as predicted by FSDT and IFSDT are suﬃciently accurate as compared to those of elasticity theory. In addition, the slight diﬀerences observed between the ﬁrst-order theories and the elasticity theory in predicting B2 have no considerable eﬀects on the interlaminar stress distributions within various laminates. The interlaminar stress components are depicted in Figs. 2 and 3 for thermal problems of cross-ply [90/0/0/90] and [0/90/0/90] laminates subjected to the boundary conditions (47) at y = ±b. It Table 1 Numerical value of the constant parameter B2 · 106 according to FSDT, IFSDT, LWT, and elasticity theory for special boundary conditions in Eqs. (47) P=1

P=2

P=3

P=4

P=5

P=6

P=7

P=8

[90/0/0/90] Layerwise theory Elasticity theory IFSDT

1.7296 1.6817 1.7876

1.6980

1.6906

1.6871

1.6852

1.6840

1.6833

1.6828

[0/90/0/90] Layerwise theory Elasticity theory FSDT

1.6633 1.6051 1.5389

1.6234

1.6252

1.6113

1.6093

1.6080

1.6072

1.6067

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8133

Fig. 2. Distribution of interlaminar stresses near the middle plane of [0/90/0/90] laminate and in the top 90 layer.

Fig. 3. Distribution of interlaminar stresses near 90/0 interface of [90/0/0/90] laminate and in the top 90 layer.

is observed that the results of the layerwise theory are in excellent agreements with those of the elasticity theory. The free-edge-eﬀect problems are now examined by using several numerical examples. The numerical values of the unknown constant parameters appearing in various displacement ﬁelds are presented for cross-ply, symmetric, and antisymmetric angle-ply laminates in Table 2. The results are generated for various width to thickness ratios. Close examination of Table 2 reveals that the FSDT and IFSDT results are suﬃciently accurate Table 2 Unknown constants of displacement ﬁeld according to FSDT and LWT Laminate

Theory

Constants

2b/h = 5

2b/h = 10

2b/h = 20

[90/0/0/0]

FSDT

B2 B6 B2 B6 B2 B2 B2 B2 B1 B2 B1 B2

7.7625e7 1.7317e3 7.6235e7 1.7197e3 1.5323e6 1.5141e6 1.8309e6 1.7793e6 5.5921e3 8.6592e7 5.5468e3 7.9602e7

7.7625e7 1.7317e3 7.7038e7 1.7274e3 1.5472e6 1.5386e6 1.9222e6 1.8970e6 5.5921e3 8.6592e7 5.5725e3 8.3327e7

7.7625e7 1.7317e3 7.7697e7 1.7358e3 1.5546e6 1.5511e6 1.9672e6 1.9577e6 5.5921e3 8.6592e7 5.5826e3 8.5260e7

LWT [90/0/0/90] [45/10/10/45] [45/10/10/45]

IFSDT LWT IFSDT LWT FSDT LWT

8134

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

for thin to moderately thick laminates. For thick laminates, however, numerical investigation indicates that slight inaccuracy in global terms (i.e., terms involving the unknown parameters B1, B2, and B6 appearing in (4)) has insigniﬁcant eﬀects on the accuracy of stress distributions within various laminates. It is, therefore, concluded here that the explicit expressions obtained for these parameters according to ﬁrst-order theories (i.e., relations (30), (31), and (32) for symmetric, cross-ply, and antisymmetric angle-ply laminates) may conveniently be used within other theories such as LWT and elasticity theory (see also Nosier and Bahrami, 2006, 2007). This, in fact, is done here in the remaining of the present study. In order to obtain accurate results for interlaminar stresses, each physical layer is subdivided into, unless otherwise mentioned, 20 numerical layers (i.e., p = 20). Moreover, the ratio of width to thickness is assumed to be 10 (i.e., 2b/h = 10). It is to be noted that for symmetric cross-ply laminates either relation (30) or (31) may be used to determine the single constant parameter B2 (noting that B6 = 0 for symmetric laminates). Fig. 4 shows the distributions of the interlaminar normal stress rz along the two 0/90 interfaces in the [0/90/0/90] laminate. It is observed that the rz exhibits diﬀerent behavior at these interfaces. More explicitly, it is seen that the maximum numerical value of rz is quite larger in the top 0/90 interface. The distributions of the interlaminar stresses rz and ryz along the upper and middle interfaces of the symmetric cross-ply [90/0/0/90] laminate are shown in Fig. 5. Both stresses are seen to grow abruptly in the vicinity of the free edge, while being zero in the interior region of the laminate. It is also noted that the interlaminar shear stress ryz rises toward the free edge and decreases rather suddenly to zero at the free edge. By increasing the number of numerical layers in each lamina ryz becomes slightly closer to zero but it may never become zero. This is, most likely, due to the fact that within LWT the generalized stress resultant Rky , rather than ryz, is forced to vanish at the free edge (see Eq. (43)). It is reminded here that

Fig. 4. Interlaminar normal stress along the two 0/90 interfaces of [0/90/0/90] laminate.

Fig. 5. Distributions of interlaminar stresses along the top and middle interfaces of [90/0/0/90] laminate.

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8135

Fig. 6. Interlaminar normal stress rz through the thickness of [90/0/90/0] laminate.

Fig. 7. Distribution of interlaminar shear stress ryz through the thickness of bottom 90 layer of [0/90/90/0] laminate.

Fig. 8. Distribution of interlaminar stresses along the 25/80 interface of [25/80/80/25] laminate.

the interlaminar shear stress rxz is identically zero everywhere in cross-ply laminates. Also, due to symmetry, the interlaminar shear stress ryz vanishes at the middle surface of symmetric cross-ply laminates. The variations of interlaminar normal stress rz through the thickness of the unsymmetric cross-ply laminate [90/0/ 90/0] are depicted in Fig. 6 as the free edge is approached. It is observed that the maximum negative value of rz occurs within the top 0 layer and the maximum positive value of rz occurs within the bottom 90 layer

8136

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

both near the 90/0 interfaces at the free edge (i.e., y = b). It is also seen that rz diminishes away from the free edge as the interior region of the laminate is approached. Fig. 7 shows the variations of transverse shear stress ryz at the free edge (i.e., y = b) and through the thickness of the bottom 90 layer of the [0/90/90/0] laminate. It is clear from the ﬁgure that ryz has a nonzero value at the interface-edge junction (i.e., interface corner) of the laminate. A close examination of Fig. 7 reveals that, except for the interface corner point, the value of ryz along the free edge of the laminate approaches zero as the number of numerical layers in each physical ply, p, is increased. The variations of the interlaminar normal and shear stresses along the upper interface (i.e., the 25/80 interface) of the antisymmetric angle-ply laminate [25/80/80/25] are plotted in Fig. 8. It is seen that the magnitude of ryz is quite smaller than those of rz and rxz (with rxz and rz surprisingly having similar magnitudes). It is reminded here that extensive numerical studies indicate that the interlaminar shear stress ryz is equal to zero at the middle surface of all antisymmetric angle-ply laminates subjected to uniform hygrothermal loads. The distributions of interlaminar stresses rz and rxz across the 0/60 interfaces of [60/ 0/0/60] and [0/60/60/0] laminates are compared in Fig. 9a and b. It is observed that both transverse normal stress rz and transverse shear stress rxz exhibit similar behavior in the two laminates. The maximum interfacial values for both rz and rxz occur, however, in the [0/60/60/0] laminate. The distributions of through-the-thickness interlaminar normal stress rz at y = b for the antisymmetric angle-ply laminate [45/ 60/60/45] and the symmetric laminate [45/60/60/45] are shown in Fig. 10. It is observed that the value of rz at the free edge is noticeably larger in the antisymmetric angle-ply laminate. The maximum value of rz in the [45/60/60/45] laminate occurs at the middle surface while the maximum value of rz in [45/ 60/60/45] occurs in the 60 layers near the top and bottom interfaces. It is to be noted that, in both symmetric and antisymmetric angle-ply laminates, the interlaminar normal stress rz is an even function of thickness coordinate. Similarly, the variations of interlaminar shear stress rxz through the thickness and at the free edge of the [(45/45)2] and [45/45]s laminates are presented in Fig. 11. It is noticed from this ﬁgure that

Fig. 9. (a) Interlaminar normal stress rz along the 0/60 interfaces of [60/0/0/60] and [0/60/60/0] laminates. (b) Interlaminar shear stress rxz along the 0/60 interfaces of [60/0/0/60] and [0/60/60/0] laminates.

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8137

Fig. 10. Distributions of interlaminar normal stress rz through the thickness of [45/60/60/45] and [45/60/60/45] laminates.

Fig. 11. Distributions of interlaminar shear stress rxz through the thickness of [(45/45)2] and [45/45]s laminates.

in the antisymmetric angle-ply laminate the maximum positive values of rxz occur near the 45/45 interfaces whereas the maximum negative value of rxz occurs at the middle surface of the laminate. In the symmetric laminate, however, the maximum positive and negative values of rxz occur near the 45/45 and 45/45 interfaces, respectively. It is signiﬁcant to note that the magnitudes of maximum values of rxz for both laminates are approximately equal, with rxz being an odd (even) function of thickness coordinate in symmetric (antisymmetric angle-ply) laminates. Finally, the eﬀect of ﬁber orientation is examined in Fig. 12a and b by comparing the variations of interlaminar normal stress rz at the top interface-edge and middle surface-edge junctions of the [0/h/h/0] and [0/ h/h/0] laminates as a function of h. It is observed that at the top interface-edge (i.e., 0/h interface-edge) junctions the two laminates display very similar behavior, with the numerical values of rz being approximately identical. At the middle surface-edge junction, however, the distributions of rz in the two laminates are, except for small h’s, quite diﬀerent. The maximum values of rz at the top interface-edge junction occur at h = 90 in both laminates whereas at the middle surface-edge junction rz becomes maximum when h 55 in the antisymmetric angle-ply laminate and when h = 90 in the symmetric laminate. 4. Conclusions In the present investigation an elasticity formulation is presented for the displacement ﬁeld of a long generally stacked laminate subjected to hygrothermal loads. It is found that the components of the displacements

8138

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

Fig. 12. (a) Interlaminar normal stress rz at the top interface-edge junctions (i.e., 0/h interface-edge junctions) of the [0/h/h/0] and [0/h/ h/0] laminates as a function of h. (b) Interlaminar normal stress rz at the middle interface-edge junctions of the [0/h/h/0] and [0/h/h/ 0] laminates as a function of h.

ﬁeld are composed of two distinct parts, signifying the global and local deformations within laminates. Based on physical arguments regarding the behavior of symmetric, cross-ply, and antisymmetric angle-ply laminates special displacement ﬁelds are obtained for such laminates. The ESL theories are then employed to determine the unknown constant parameters appearing in the global deformation part of various displacement ﬁelds. It is also found that for each lamination scheme an appropriate ESL theory must be employed for the eﬃcient and accurate prediction of these parameters. For cross-ply and antisymmetric angle-ply laminates it is found that the usual ﬁrst-order theory (Mindlin–Reissner plate theory) yields accurate results for the unknown constant parameters appearing in various displacement ﬁelds. Numerical investigations, however, reveal that for symmetric laminates the usual ﬁrst-order theory (FSDT) is inadequate in predicting these parameters. Therefore, an improved ﬁrst-order theory (IFSDT) is introduced to obtain these parameters for symmetric laminates. Next, Reddy’s layerwise theory (LWT) is utilized to calculate the interlaminar stresses. The unknown constants appearing in various displacement ﬁelds are also determined within LWT. For special boundary and loading conditions an analytical elasticity solution is presented to verify the accuracy of LWT, in predicting the interlaminar stresses and B2, and that of FSDT and IFSDT in predicting B2. Excellent agreements are seen to exist between the results of LWT and the elasticity theory. Several numerical results according to LWT are then developed for the free-edge interlaminar stresses through the thickness and across the interfaces of various cross-ply, symmetric, and antisymmetric angle-ply laminates. Appendix A 22 , D 26 , and D 66 appearing in (26) are given as follows: The coeﬃcients D

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

~ ~ ~ ~ ~ ~ 22 ¼ D22 þ B26 ðA26 B22 A22 B26 Þ þ B22 ðA26 B26 A66 B22 Þ D 2 A22 A66 A26 ~ ~ ~ ~ ~ ~ 26 ¼ D26 þ B26 ðA26 B26 A22 B66 Þ þ B22 ðA26 B66 A66 B26 Þ D 2 A22 A66 A26 ~ ~ ~ ~ ~ ~ 66 ¼ D66 þ B66 ðA26 B26 A22 B66 Þ þ B26 ðA26 B66 A66 B26 Þ : D 2 A22 A66 A26 The constant parameters in Eqs. (28a) and (28b) are deﬁned as: 1 16 a4 B 12 ; a3 B 12 a1 B 16 Þ ða2 B a1 a4 a2 a3 1 T a2 M T ; a1 M T a3 M TÞ ða4 M ðmTy ; mTxy Þ ¼ y xy xy y a1 a4 a2 a3 1 H H a2 M H ; a1 M H a3 M HÞ ðmH ða4 M y ; mxy Þ ¼ y xy xy y a1 a4 a2 a3 ðd 1 ; d 2 Þ ¼

where 22 Þk1 coshðk1 bÞ; 26 þ D 1D a1 ¼ ð D 26 Þk1 coshðk1 bÞ; 66 þ D 1D a3 ¼ ð D

22 Þk2 coshðk2 bÞ 26 þ D 2D a2 ¼ ðD 26 Þk2 coshðk2 bÞ 66 þ D 2D a4 ¼ ðD

~ ~ 12 ¼ B ~ 12 þ B26 ðA12 A26 A16 A22 Þ þ B22 ðA16 A26 A12 A66 Þ B A22 A66 A226 ~ ~ 16 ¼ B ~ 16 þ B66 ðA12 A26 A16 A22 Þ þ B26 ðA16 A26 A12 A66 Þ B A22 A66 A226 and T ¼M ~T M y y

~ 26 ðA22 N T A26 N T Þ þ B ~ 22 ðA66 N T A26 N T Þ B xy y y xy

T ¼ M ~T M xy xy H ¼M ~H M y y H ¼ M ~H M xy xy

A22 A66 A226 ~ 66 ðA22 N T A26 N T Þ þ B ~ 26 ðA66 N T A26 N T Þ B xy y y xy A22 A66 A226 ~ 26 ðA22 N H A26 N H Þ þ B ~ 22 ðA66 N H A26 N H Þ B xy y y xy A22 A66 A226 ~ 66 ðA22 N H A26 N H Þ þ B ~ 26 ðA66 N H A26 N H Þ B xy y y xy A22 A66 A226

:

In addition, the constant coeﬃcients appearing in (30) are deﬁned as follows: ^ 11 b þ d 1 ðB 1 Þ sinhðk1 bÞ þ d 2 ðB 2 Þ sinhðk2 bÞ 16 þ B 12 D 16 þ B 12 D h¼A 1 Þ sinhðk1 bÞ mT ðB 2 Þ sinhðk2 bÞ T mT ðB 16 þ B 12 D 16 þ B 12 D nT ¼ b N x

nH x

x

y

xy

1 Þ sinhðk1 bÞ mH ðB 2 Þ sinhðk2 bÞ H mH ðB 16 þ B 12 D 16 þ B 12 D ¼ bN x y xy

where 11 ¼ A11 þ A16 ðA12 A26 A16 A22 Þ þ A12 ðA16 A26 A12 A66 Þ A A22 A66 A226 and

8139

8140

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

T ¼ NT N x x

A16 ðA22 N Txy A26 N Ty Þ þ A12 ðA66 N Ty A26 N Txy Þ

H ¼ NH N x x

A22 A66 A226 H H H A16 ðA22 N H xy A26 N y Þ þ A12 ðA66 N y A26 N xy Þ

A22 A66 A226

:

Appendix B The constant coeﬃcients appearing in (31) are given as follows: h1 ¼ A11 a1 þ A12 a2 þ B12 a3 ; h3 ¼ B11 a1 þ B12 a2 þ D12 a3 ;

h2 ¼ B11 a1 þ A12 a4 þ B12 a5 h4 ¼ D11 a1 þ B12 a4 þ D12 a5

nTx ¼ N Tx a1 þ N Ty a2 þ M Ty a3 ;

mTx ¼ M Tx a1 þ N Ty a4 þ M Ty a5

and

H H H nH x ¼ N x a1 þ N y a 2 þ M y a3 ;

H H H mH x ¼ M x a1 þ N y a4 þ M y a5

where a1 ¼ A22 D22 B222 ; a2 ¼ B12 B22 A12 D22 ; a3 ¼ A12 B22 A22 B12 a4 ¼ B22 D12 B12 D22 ; a5 ¼ B12 B22 A22 D12 : It is reminded here that the laminate rigidities and stress, thermal, and hygroscopic resultants are the same as those deﬁned in Eqs. (19), (21), (22), and (23). Furthermore, here: Z h=2 11 ; Q 12 Þax þ ðQ 12 ; Q 22 Þay DTz dz ðM Tx ; M Ty Þ ¼ ½ðQ h=2

H ðM H x ; My Þ ¼

Z

h=2

11 ; Q 12 Þbx þ ðQ 12 ; Q 22 Þby DMz dz ½ðQ

h=2

and Bij ¼

Z

h=2

ij z dz: Q

h=2

It is observed that the constant parameters B2 and B6 appearing in (31) are independent of shear correction factor. In other words, the results presented in (31) for B2 and B6 are also obtainable from the classical lamination theory. Appendix C The constant coeﬃcients appearing in (32) are given by: h1 ¼ 2ðA12 B26 A22 B16 Þ h2 ¼ A11 A22 A212 h3 ¼ 2ðB226 A22 D66 Þ h4 ¼ A22 B16 A12 B26 and

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

8141

nTx ¼ A22 N Tx A12 N Ty mTxy ¼ A22 M Txy B26 N Ty H H nH x ¼ A22 N x A12 N y H H mH xy ¼ A22 M xy B26 N y

where M Txy

¼

MH xy ¼

Z

h=2

16 ax þ Q 26 ay þ Q 66 axy DTz dz ½Q

h=2

Z

h=2

16 bx þ Q 26 by þ Q 66 bxy DMz dz ½Q

h=2

with the remaining thermal and hygroscopic resultants being the same as those deﬁned in (22a) and (23a). For antisymmetric angle-ply laminates the results in (32) may also be arrived at by using the classical lamination theory. Appendix D The laminate rigidities, introduced in (40), are given as follows (also see Nosier and Bahrami, 2006, 2007): 8 ðk1Þ ðk1Þ ðk1Þ > C C hk1 C pq pq pq > ; ; if j ¼ k 1 > > hk1 2 6 > > > > > C ðk1Þ C ðkÞ C ðk1Þ C ðkÞ h C ðk1Þ h C ðkÞ > < pq þ pq ; pq pq ; k1 pq þ k pq if j ¼ k kj kj hk1 hk 2 2 3 3 ðAkj ; B ; D Þ ¼ pq pq pq > > > ðkÞ ðkÞ ðkÞ C C hk C > pq pq pq > ; ; if j ¼ k þ 1 > > hk 2 6 > > > : ð0; 0; 0Þ if j < k 1 or j > k þ 1 and

8 h3 3 i 2 2 ð1Þ ð1Þ z21 z22 > ð1Þ h1 C pq ð1Þ z1 z2 C pq z1 z2 > C pq ; 2 ; C pq 2h1 ; h1 z2 2 > 3 > > > >

> h3 3 i > ðk1Þ ðk1Þ > zk zk1 z2k z2k1 C z2k z2k1 hk1 C pq pq ðk1Þ ðk1Þ > > ; C pq ; hk1 zk1 2 < C pq ; 2 2hk1 3 k ; Dk Þ ¼ ðAkpq ; Bkpq ; B pq pq ðk1Þ ðkÞ 2 2 2 2 > > ðkÞ ; hk1 C pq þ hk C pq ; C ðk1Þ zk zk1 þ C ðkÞ zk zkþ1 ; ðk1Þ C > C > pq pq pq pq 2 2 2h 2h > k k1 > > > > ðk1Þ h 3 3 i h i ðkÞ > 3 3 2 2 2 2 z z > z z z z z z C C > : hpqk1 k 3 k1 zk1 k 2 k1 þ hpqk k 3 kþ1 zkþ1 k 2 kþ1

if k ¼ 1 if k ¼ N þ 1

if 1 < k < N þ 1:

References Cho, M., Kim, H.S., 2000. Iterative free-edge stress analysis of composite laminates under extension, bending, twisting and thermal loadings. International Journal of Solids and Structures 37 (3), 435–459. Fung, Y.C., Tong, P., 2001. Classical and Computational Solid Mechanics. World Scientiﬁc, New Jersey. Herakovich, C.T., 1998. Mechanics of Fibrous Composites. John Wiley & Sons, New York. Jones, R.M., 1998. Mechanics of Composite Materials. Taylor & francis, London. Kant, T., Swaminathan, K., 2000. Estimation of transverse/interlaminar stresses in laminated composites-a selective review and survey of current developments. Composite Structures 49, 65–75. Kassapoglou, C., Lagace, P.A., 1986. An eﬃcient method for the calculation of interlaminar stresses in composite materials. Journal of Applied Mechanics 53, 744–750. Kassapoglou, C., Lagace, P.A., 1987. Closed form solutions for the interlaminar stress ﬁeld in angle-ply and cross-ply laminates. Journal of Composite Materials 21 (1), 292–308.

8142

A. Bahrami, A. Nosier / International Journal of Solids and Structures 44 (2007) 8119–8142

Kim, T., Atlury, S.N., 1995. Analysis of edge stresses in composite laminates under combined thermo-mechanical loading using a complementary energy approach. Computational Mechanics 16, 83–87. Lekhnitskii, S.G., 1981. Theory of Elasticity of an Anisotropic Body. Mir Publishers. Matsunaga, H., 2004. A Comparison between 2-D single-layer and 3-D layerwise theories for computing interlaminar stresses of laminated composite and sandwich plates subjected to thermal loadings. Composite Structures 64, 161–177. Morton, S.K., Webber, J.P.H., 1993. Interlaminar failure due to mechanical and thermal stresses at the free edges of laminated plates. Composite Science and Technology 47, 1–13. Nosier, A., Bahrami, A., 2006. Free-edge stresses in antisymmetric angle-ply laminates in extension and torsion. International Journal of Solids and Structures 43, 6800–6816. Nosier, A., Bahrami, A., 2007. Interlaminar stresses in antisymmetric angle-ply laminates. Composite Structures 78, 18–33. Nosier, A., Kapania, R.K., Reddy, J.N., 1993. Free vibration analysis of laminated plates using a layerwise theory. AIAA Journal 13 (12), 2335–2346. Pagano, N.J., 1974. On the calculation of interlaminar normal stress in composite laminate. Journal of Composite Materials 8, 65–81. Pipes, R.B., Pagano, N.J., 1970. Interlaminar stresses in composite laminates under uniform axial extension. Journal of Composite Materials 4, 538–548. Reddy, J.N., 2003. Mechanics of Laminated Composite Plates and Shells: Theory and Analysis. CRC Press, New York. Rohwer, K., Rolfes, R., Sparr, H., 2001. Higher-order theories for thermal stresses in layered plates. International Journal of Solids and Structures 38, 3673–3687. Tahani, M., Nosier, A., 2003. Free edge stress analysis of general cross-ply composite laminates under extension and thermal loading. Composite Structures 60, 91–103. Tahani, M., Nosier, A., 2004. Accurate determination of interlaminar stresses in general cross-ply laminates. Mechanics of Advanced Materials and Structures 11 (1), 67–92. Wang, A.S.D., Crossman, F.W., 1977a. Some new results on edge eﬀect in symmetric composite laminates. Journal of Composite Materials 11, 92–106. Wang, A.S.D., Crossman, F.W., 1977b. Edge eﬀects on thermally induced stresses in composite laminates. Journal of Composite Materials 11, 300–312. Wang, S.S., Choi, I., 1982. Boundary-layer hygroscopic stresses in angle-ply composite laminates. AIAA Journal 20 (11), 1592–1598. Wang, Y.R., Chou, T.W., 1989. Three-dimensional transient interlaminar stresses in angle-ply composites. Journal of Applied Mechanics 56, 601–608. Webber, J.P.H., Morton, S.K., 1993. An analytical solution for the thermal stresses at the free edges of laminated plates. Composite Science and Technology 46, 175–185. Yin, W.L., 1997. The eﬀect of temperature gradient on the free-edge interlaminar stresses in multilayered structures. Journal of Composite Materials 31 (24), 2460–2477.

Copyright © 2021 COEK.INFO. All rights reserved.